Volume 9, No. 27, Sept. 2015, pages 106–111
DOI: 10.12913/22998624/59091 Research Article
Received: 2015.07.15 Accepted: 2015.08.05 Published: 2015.09.01
INFLUENCE OF PIEZOELECTRIC TRANSDUCER TO GLASS FIBER
REINFORCED COMPOSITE STIFFNESS
Witold Rządkowski1, Karol Suprynowicz1, Paweł Pyrzanowski1
1 Faculty of Power and Aeronautical Engineering, Institute of Aeronautics and Applied Mechanics, Warsaw
University of Technology, Nowowiejska 24, 00-665 Warsaw, Poland, e-mail: email@example.com; firstname.lastname@example.org; email@example.com
The main goal was to determine if transducers based on piezoelectric materials are suitable for strain calculations in thin GFRP specimens. Numerous experimental studies, both physical and numerical, performed by the authors, have shown that there is a huge influence of bonded piezoelectric transducer on the overall stiff -ness of the measured object. The paper presents tensile test performed on strength machine with Digital Image Correlation strain and deflection observations. Test were compared with FEM models for detailed investigation. The main conclusion is piezoelectric transducers has huge influence on local stiffness of measured object. That is critical especially when they are used as strain sensors, when presence of sensor is influencing to measured results.
Keywords: piezo material, stiffness, piezoelectric strain sensor.
In recent years piezoelectric materials are in-creasing their share in multiple fields of engineer -ing applications. Their main advantage in sensor mode, when due to external excitation electric charge is generated, is independence from external power sources. Very high stiffness of piezoelectric ceramic materials gives in result very small de-formations when load is applied. This results in a high resonance frequency, which, generally, is very desired in dynamic applications. Thereby they are very suitable for high frequency and impact load registration. On the other hand, it is hard to use them in small frequency load observations, due to electrical drift and energy dissipation by amplifiers.
The most important property due to reverse inverse piezoelectric effect is possibility to use them as actuators, where in combined sensor-ac-tuator mode they can work as intelligent dumping  or adaptive wing geometry systems 
The most common used piezoelectric materi-al PZT besides many advantages as high mechan -ical-electrical coupling factor, high permittivity
and piezoelectric charge coefficient, they have also disadvantages like high fragility. They can be embedded inside composite structure to monitor the stress/strain concentration levels at the critical locations  or to delamination detection . On the other hand, it is hard to use them in small fre-quency load observations, due to electrical drift and energy dissipation by amplifiers . In that case also high stiffness may be undesired prop-erty, especially when thick and no so rigid struc-tures are monitored. In this paper investigation of piezo transducer for local strain distribution and global stiffness of GFRP probes is presented.
Research objective was to determine the in-fluence of piezo sensor on stiffness of GFRP probes. Strain measurements obtained on piezo transducer also have to be investigated, when lo-cally strain values are influenced by that sensor.
3 layers of glass fabric. Reinforcement consist of 186 g/m2 glass fabric and epoxy EP52 was used as a matrix.
Also a probe from aluminum alloy was pre-pared as a reference, due isotropic material prop-erties. On all the probes MFC (Macro Fiber Com -posite) M2807-P1(28×7×0.1mm) and resistive strain gauge with active area 30×3.8 mm were bonded. Simple tension test were performed on Instron strength machine and all results were reg-istered with National Instruments data acquisition system. Nikon digital camera with open source software prepared by Karol Suprynowicz . On Figure 1 reference, aluminum alloy specimen with bonded transducers, before DIC markers ap-plication is presented.
Schematic represantation of fabric orirntation is shown on Figure 2. Overall stiffness of speci -men is the highes for PPP samples, and lowest for
described as SSS. When both piezo and resistive gauge transducers are bonded DIC markers were applied. Sub-pixel, two dimensional DIC  was used to determine stain distribution and for at-taching virtual extensometrs
TESTS AND RESULTS
Simple tension test were performed, where applied deflection was 0.85 mm. Strain calculated from the formula:
is equal to 0.2125%, when l0 is 400 mm and is very similar as calculated on DIC extensometer, when extensometer is applied above piezo sensor. It is worth to see that deflection at the end point and all intermediate points are consistent. Deflec -tions at end point are presented on Figure 4.
Deflection along Y axis is very close to theo -retical in every region of specimen and no sig-nificant disruption is observed. Locally there is a strain concentration observed on the area of MFC transducer. Vertical (Y) strain results for speci -men PPP are presened on Figure 5.
Fig. 1. Tested specimen
Fig. 2. Fabric orientation: P – fabric layer with 0/900
orientation, S – fabric layer with -45/450 orientation
The calculated strain values in the area of piezo sensor are significantly lower than those calculated from the analytical formulas and cal-culated by DIC in the area above the sensor. Two points below MFC transducer, where strain is also lower there are soldering points that should not be taken into consideration.
When displacements are also taken into con-sideration it leads to a conclusion that stiffness is locally higher, if deflections are continuous and strains are lower.
Numeric test were also performed for de-tailed investigation. FEM model has not the same geometric properties as the model used in the test, because FEM model was prepared to test new design of piezo actuator , but the influ -ence of piezo material for local and global stiff-ness is also easy to show. According to greater piezo thickness in FEM model (0.8 mm in FEM vs. 0.3 mm in experiment) that influence should be even more easily noticeable. In Figure 6 the results of strain i vertical direction (y) are present -ed. On the left the results for the side with bonded piezo transducer are shown and on the right of the opposite side. It is easy to observe that local strain distribution is highly disrupted in the surrounded area of the piezo transducer. On second side this influence is still visible, but it is not so huge as on the front side.
PPP probes are the stiffest when they are loaded in Y direction, and stiffness drops when S layers number increased. The results for speci-men SSS – less stiff in tension (Y) direction are presented on Figure 7.
Strain values in the area of piezo transducer in SSS samples measured by DIC method are lower than for PPP probes. It is easier to de-termine if the results are combined together. In
Fig. 5. Vertical (Y) strain in PPP specimen
Fig. 6. Vertical (Y) strain in PPP specimen on front(left side) and back (right side)
Fig. 7. Vertical (Y) strain in SSS specimen
Figure 8 the measurements from middle of load cycle are presented.
The amount of strain field in yellow and green color is higher in SSS probe, but it is necessary to take deflection distribution in SSS sample into consideration, which are shown in Figure 9.
Deflection distribution in SSS sample is the same as in PPP sample. So the only reasonable justification is local stiffness change in the area of sensor. That change has not only a result in starain maps in probes, it also influences the ob -tained strain values from piezo sensor. The re-Fig. 9. Vertical (Y) deflection in PPP and SSS
Fig. 10. Voltage values in 4 types of samples
sults from FEM calculations for 4 types of fabric orientation are shown on Figure 10.
Results shown clearly prove that presence of piezoelectric sensor has an influence on volt -age vales obtained from piezo transducer. That voltage is dependent from strain, and presence of sensor effects that value.
It is worth to compare strain distributions in all types of specimens and investigate with probe without bonded piezoelectric transducer. In Figure 11 such results are presented. It is worth to notice that the last one (PPP without MFC) has almost constant strain distribution. Only distortion is present at ends, and is caused by boundary conditions applied in that areas. Degrees of freedom are locked at ends to simu-late clamping in strength machine. In that case specimens were load by 0.05 mm displacement, and their overall length was 150 each. Theo-retical strain calculated from e=∆l/l0 formula is equal to 0.33‰.
Both voltage values from Figure 10 and strain values from Figure 11 are summarized in the plot below. Figure 12 is a chart of both strains on the front and back of specimens with obtained voltage values (right Y axis). Of course, functions are not linear, due to nonlin-ear behavior of specimens. Bonded piezoelec-tric sensor changes locally location of neutral bending plane.
Piezoelectric materials are very interesting and useful for engineers. They can be used in many fields of modern engineering. Strain sensor is one of such use, but in that case special precau-tions must be taken. Piezoelectric transducers can significantly change the stiffness of the measured probes, and decrease the obtained strain values causing that the results are unreliable. This situa-tion was observed in laboratory tests and confirmed by numerical calculations. The best solution can be made to prevent that situation – the results can be scaled by a factor to match strain values in the area not in close region to the sensor. Such an approach requires additional method to calculate real strains and in many applications it becomes unreason-able. This and other difficulties, like output signal drop in time in low frequency loads, makes sensors based on piezoelectric ceramics material are still no first choice in strain measurements.
Financial support of Structural Funds in the Operational Programme – Innovative Economy (IE OP) financed from the European Regional Devel -opment Fund – Project “Modern material technol-ogies in aerospace industry”, No POIG.01.01.02-00-015/08-00 is gratefully acknowledged.
1. Paradies R., Ciresa P., Active wing design with integrated flight control using piezoelectric macro fiber composites. Smart Materials and Structures, 2009.
2. Debiasi M., Leong C.W., Boureme Y., Yen Y.C., Application of Macro-Fiber-Composite Mate-rials on UAV, 2013, online March 2015, http:// www.marcodebiasi.net/MDresearch/MDpublica --tions/2013ATS-Paper-MFCwingShaping.pdf] 3. Konka H.P., Wahab M.A., Lian K., Piezoelectric
fiber composite transducers for health monitoring in composite. Sensor and Actuators A, 194, 2013, 84–94.
4. Yeum C.M., Sohn H., Ihn J.B., Lim H.J., Instanta -neous delamination detection in a composite plate using a dual piezoelectric transducer network. Composite Structures, 94, 2012, 3490–3499.
5. Rządkowski W., Pyrzanowski P., Determination of damage to the piezoelectric sensor by measuring the electrical capacitance. Solid State Phenomena, Warsaw 2015.
6. Suprynowicz K., Kowalik M., Obszański M., Rządkowski W., Pyrzanowski P., Estimation of piezoelectric strain sensor influence on glass fiber reinforced composite sample’s stiffness using digi-tal image correlation. In: 30th Danubia Adria Sym-posium on Advenced Mechanics, Croatia 2013, 105–106.
7. Bruck H.A., McNeill S.R., Sutton M.A., Peters III W.H., Digital image correlation using Newton-Rap-son method for partial differential correction. Smart Structures and Intelligent Systems, 1993, 341–352. 8. Pyrzanowski P., Rządkowski W., Suprynowicz